DOI: http://dx.doi.org/10.1590/1516-1439.019015Materials Research. 2015; 18(3): 608-613 2015
1. IntroductionDuring the recent years, intensive research activity has
been focused on mesoporous materials like MCM-411-6. The MCM-41 shows no considerable acidity, limiting their direct use in catalytic reactions. However, due to its high specific area, they are excellent catalyst supports, which can generate acid/base sites during or after synthesis either by impregnation or by isomorphous substitution of heteroatom in the MCM-41, especially metals incorporation such as Al, Ti, Zr, B, V, etc7. The introduction of titanium in MCM-41 was reported for the first time in 19948. The iso and nonisomorphic substitutions usually enhance catalytic activity in processes of commercial interest such as: hydrocarbon catalytic cracking isomerization, hydrodesulphurization, oxidation reactions, hydroxylation and epoxidation of aromatics, olefins and phenols9.
Many authors10-12 have used the rice husk ash (RHA) as silica source in the synthesis of various mesoporous
materials (ZSM-5, MCM-41, MCM-48, SBA-15) using different extraction methods of silica. This agricultural waste has attracted great interest from researchers due to its high silicon content (>90%) of low cost that can be use as Si source in different silica based materials.
The synthesis of Ti-MCM-41 takes place by mixing the silica source and template, which is usually a long-chain surfactant that give micelles, which originate tubes forming hexagonally ordered structure characteristic of MCM-41. The gel prepared with these reagents at different molar ratios surfactant/silicon is subjected to a hydrothermal treatment in alkaline conditions, then washed and dried at room temperature. The template removal, which occur by calcination at approximately 550 C, results in a silicon material of high specific area and large diameters porous.The synthesis conditions can be changed with the purpose of obtaining materials with different properties. The factors affecting the final product are molar ratio template/silica
Comparison of Kinetic Study of CTMA+ Removal of Molecular Sieve Ti-MCM-41 Synthesized with Natural and Commercial Silica
Maria do Socorro Braga Fontesa*, Dulce Maria de Arajo Melob, Cintia de Castro Costac,
Renata Martins Bragad, Marcus Antonio de Freitas Meloe, Jos Antnio Barros Leal Reis Alvesf
aPrograma de Ps-Graduao em Cincia e Engenharia de Materiais PPGCEM, Universidade Federal do Rio Grande do Norte UFRN, Campus Universitrio Lagoa, Natal, RN, Brazil
bDepartamento de Qumica, Universidade Federal do Rio Grande do Norte UFRN, Natal, RN, BrazilcPrograma de Ps-Graduao em Cincia e Engenharia de Petrleo PPGCEP,
Universidade Federal do Rio Grande do Norte UFRN, Natal, RN, BrazildEscola Agrcola de Jundia EAJ, Universidade Federal do Rio Grande do Norte UFRN,
Macaba, RN, BrazileDepartamento de Engenharia Qumica, Universidade Federal do Rio Grande do Norte UFRN,
Natal, RN, BrazilfDepartamento de Qumica, Universidade Federal do Rio Grande do Norte UFRN, Natal, RN, Brazil
Received: April 1, 2015; Revised: April 28, 2015
This work aimed to determine and compare the apparent activation energy, involved in thermal decomposition of CTMA+ from the pores of Ti-MCM-41 synthesized by two different source of silica in order to evaluate their influence in the template removal. The molecular sieves Ti-MCM-41 were synthesized using rice husk ash (RHA), as alternative low cost source of silica, and commercial silica gel, obtaining two mesoporous material by hydrothermal synthesis of gel molar composition of: 1.0 CTMABr: 4.0 SiO2: X TiO2: 1.0 Na2O: 200.0 H2O. The samples were characterized to compare its properties by X-ray diffraction, IR spectroscopy, BET method and thermogravimetric analysis (TGA). The kinetic study using the model proposed by Flynn and Wall to determine the apparent activation energy for CTMA+ removal was performed using TGA data. The thermogravimetric analysis results of the material obtained from RHA confirmed intrinsic properties of mesoporous MCM-41 as the synthesized with commercial silica gel, such as high specific area, mesoporous range of pore diameter and hexagonal structure. According to the kinetics results the RHA showed similar chemical interaction to commercial silica gel, which makes it an interesting material, since it is a low cost source of natural silica from agricultural waste.
Keywords: Ti-MCM-4, rice husk ash, molecular sieve, kinetic
2015; 18(3) 609Comparison of Kinetic Study of Ctma+ Removal of Molecular Sieve Ti-Mcm-41 Synthesized
with Natural and Commercial Silica
concentration and length of the carbon chain of the template, synthesis temperature, pH and nature of silica13.
This work aims the use of the rice husk ash (RHA) and commercial silica gel (SG) as alternatives source of silica in the synthesis of Ti-MCM-41, performing the kinetic study of surfactant cetyltrimethyl ammonium bromide (CTMA+) removal, using the model proposed by Flynn-Wall, trough thermogravimetric analysis data, relating the apparent activation energy with the chemical interaction of silica sources and the template CTMA+ used in synthesis of this material.
2. Experimental Procedure2.1. Silica extraction
The rice husk (RH) collected at Rio Grande do Norte State, northeast of Brazil was washed in hot water 60 C, under constant stirring for 1 h, dried at 100 C for 12 h. After it was crushed in a knife mill (TECNAL TE 631), sieved at 150 mesh (0.106 mm) and calcined in a muffle furnace (TECNAL 3000) at 600 C, de 10 C min1 for 2 h. The resultant material (RHA) was used as silica source in the synthesis of Ti-MCM-41.
2.2. Hydrothermal synthesisThe synthesis of the molecular sieve MCM-41 was
conducted hydrothermally from molar ratio of 1.0 CTMABr: 4.0 SiO2: X TiO2: 1.0 Na2O: 200.0 H2O. The X value was set to the molar ratio Si/Ti equal to 50. The silica dispersion and CTMABr solution was submitted to stirring for 1 h and transferred to a stainless steel autoclave heated in an oven at 100 C for 5 days. The pH correction were made daily in the range 910 with a 30% acetic acid solution until it reach stability. The material was filtered and washed with a 2% solution of HCl in ethanol and then with distilled water. The material resulting from the crystallization process was dried at 100 C for 4 h. Finally, the solid resulting was subjected to TGA analysis for analyze the better calcination condition according kinetic study.
2.3. CharacterizationX-ray diffraction (XRD) analyses were conducted on
equipment Shimadzu XRD-7000 using a Cu-K radiation source with voltage of 30kV, current of 30 mA and Ni filter. Data were collected in the 2 range from 1 to 10. FTIR analyses were performed using Shimadzu Fourier transform infrared spectrophotometer model IR - Prestige 21 using KBr disks. For the KBr disks preparation, the samples were dried in an oven at 100 C for 2 hours, and then mixed (2 w/w% concentration) with solid KBr, the material obtained was hydraulically pressed (Carver Press) with five tons and the disks were submitted to analysis, whose spectra were scanned in the region from 4000 to 400 cm1. The specific area of the samples was determined by nitrogen adsorption at 77 K using the BET method in a Quantachrome NOVA 2000 instrument. Before the nitrogen measurement, samples were degassed at 300 C in helium for 3 h. The wall thickness (w) of MCM-41 was obtained by the difference between the lattice parameter a0 and the pore diameter (dp). The thermogravimetric analysis were performed in a thermobalance, model TGA-60 Shimadzu
using a nitrogen atmosphere, with a flow rate of 50 ml.min1 in the temperature range of 30 to 600 C, the heating rate of 5, 10 and 20 C min1.The UV-Vis analysis were performed in infrared spectrophotometer model Shimadzu, UV-2450.
2.4. Kinetic methodsThe kinetic study consists in determining the decomposed
fraction () as a function of reaction time (t) for processes in which the temperature is kept constant or in processes in which the temperature varies linearly with time. In thermogravimetric analysis (TGA), the fraction decomposed () is defined by Equation 1. The decomposition rate of CTMA+ from the pores of Ti-MCM-41 depends on temperature (T), conversion () and reaction time (t). In the TGA, the conversion of CTMA+ is expressed by (Equation 1).
( )( ) o t
m mm m
Where: mo is the initial mass, mf is the final mass, and mt is the Ti-MCM-41 mass, which varies with time.
The decomposition rate of CTMA+ can be expressed by Equation 2, where the reaction rate is related to the sample decomposition.
( )n1 d d K
Where K is a constant rate obtained by Arrhenius equation, (Equation 3).
/E RTK Ae= (3)
The determination of global kinetic parameters via TGA was based on method proposed by FlynnWall that involves measuring the temperature corresponding to fixed values of conversion () from experiments at different heating rates (), and plotting log () against 1/T giving straights lines with slopes -Ea/R14. This model require at least three dynamic curves with different and constant heating rates (); in this work it was assumed as 5, 10, and 20 C min1 with temperature between 30 and 900 C, mass of the samples was approximately 3 mg. This model was used to determine the apparent activation energy (Equation 4) and conversion () as a function of temperature.
( )R 1Ea log / (b T
Where is the heating rate, T is the absolute temperature (K), b is an interaction variable, R is the universal gas constant and Ea is the activation energy (J mol1).
3. Results and Discussi